## A mean ﬁeld model of dynamic and post-dynamic recrystallization

predicting kinetics, grain size and ﬂow stress

O. Beltran

a, K. Huang

b,⇑, R.E. Logé

a,b aMines ParisTech, CEMEF-Centre for Material Forming, CNRS UMR 7635, BP 207, 1 Rue Claude Daunesse, 06904 Sophia Antipolis Cedex, France b

Thermomechanical Metallurgy Laboratory – PX Group Chair, Ecole Polytechnique Fédérale de Lausanne (EPFL), CH-2002 Neuchâtel, Switzerland

a r t i c l e

i n f o

Article history: Received 5 January 2015

Received in revised form 20 February 2015 Accepted 23 February 2015

Keywords: Modeling

Dynamic recrystallization Post dynamic recrystallization Grain growth

Nucleation 304L steel

a b s t r a c t

A physically-based two-site mean ﬁeld model has been developed to describe the microstructural evolu-tion due to recrystallizaevolu-tionduringandafterdeformation. The model has been applied to predict the recrystallized fraction, recrystallized grain size, and ﬂow stress of 304L austenitic stainless steel during discontinuous dynamic recrystallization (DDRX), post-dynamic recrystallization (PDRX) and grain growth (GG). The model parameters vary with temperature and strain rate but do not depend on grain size. In PDRX and GG regime, the parameters only depend on temperature. The model responds well to conditions with different temperatures, strain rates, strains and/or annealing times. Particular atten-tion is paid to the occurrence of two-stage growth in the recrystallized grain size plots when PDRX occurs. There is a good quantitative agreement between model predictions and experimental results obtained in the different recrystallization regimes, opening the possibility of modeling multi-pass operations compatible with industrial applications.

Ó2015 Elsevier B.V. All rights reserved.

1. Introduction

Recrystallization is an important phenomenon that causes microstructural changes in deformed materials, thereby affecting its properties. Many metallic components are produced from large castings, which are then further deformed by forging, extrusion, rolling, etc., into an intermediate or ﬁnal product. Three different recrystallization behaviors are usually observed during these pro-cesses, namely, dynamic, post-dynamic and static recrystallization. The recrystallization regime depends on whether it occurs during hot deformation or between deformation intervals.

In static recrystallization (SRX), the deformation is interrupted before reaching the critical strain for dynamic recrystallization (DRX),

e

DRXcr . During this recrystallization regime, both nucleation

and growth of new grains take place during annealing periods between intervals of hot deformation. On the other hand, these processes can also be observed during deformation once

e

DRXcr is

reached, leading to dynamic recrystallization. Post-dynamic recrystallization (PDRX) refers to the growth of dynamically formed nuclei once deformation (greater than

e

DRXcr ) has come to

an end. Grain growth (GG) is deﬁned as the uniform coarsening

of a material with a minimal dislocation content at a high tempera-ture[1].

Although extensive efforts have been put on a wide range of materials, recrystallization during and following deformation is still not fully understood[2]. Experimentally, the softening fraction

[3]during annealing of dynamically recrystallized microstructures was often used to differentiate recrystallization regimes, due to the fact that it is difﬁcult to distinguish SRX and PDRX[4]. Researchers at McGill University were probably the ﬁrst ones who investigated the post-dynamic softening. They proposed a mechanism involving three different restoration processes including recovery, PDRX, and SRX, based on metallographic examination on polycrystalline cop-per[5–7]. Later, Sakai et al.[8,9]performed further research on the subject using a nickel alloy and austenitic steels, providing a detailed description of the above restoration processes. The observed fractional softening is, however, a combined effect of recovery, recrystallization and (where applicable) precipitation contributions, making it hard to distinguish their separate inﬂu-ences. The different mechanisms acting after hot deformation have been further studied by Hodgson and co-workers[10–13], while the mechanisms of recrystallization during and after deformation have been carefully examined by Dehghan-Manshadi et al.

[14,15]using 304 austenitic stainless steels.

Several models have been proposed to investigate the effect of the thermomechanical parameters on the softening kinetics during

http://dx.doi.org/10.1016/j.commatsci.2015.02.043

0927-0256/Ó2015 Elsevier B.V. All rights reserved.

⇑ Corresponding author. Tel.: +41 21 69 54472. E-mail address:ke.huang@epﬂ.ch(K. Huang).

Contents lists available atScienceDirect

## Computational Materials Science

j o u r n a l h o m e p a g e : w w w . e l s e v i e r . c o m / l o c a t e / c o m m a t s c iand after deformation, however, limited studies have been reported on the microstructural evolution in terms of recrystal-lized volume fraction and grain size. A large group of these models are based on the Johnson–Mehl–Avrami–Kolmogorov (JMAK) equation approach[15–21]. However, the ideal JMAK behavior is rarely exhibited by real materials. Such deviation from this ideal behavior is due to the presence of recovery, non-uniform dis-tribution of stored strain energy, non-random disdis-tribution of recrystallized nuclei, and anisotropic growth of the recrystallized nuclei[22]. For this category of models, experimental validation is often lacking, and good agreement between numerical and experimental data in terms of grain size is rare. Beyond the JMAK model, the evolution of dislocation density populations can be dis-cretely followed through the entire deformation process, e.g. by Roucoules et al. [23], based on the Sandstrom and Lagneborg approach[24,25]. However, in[23], the recrystallized grain size, which is of interest in most of the industrial applications, was not analyzed. It is furthermore assumed that the mechanisms which take place during dynamic and static recovery or during DRX, SRX or PDRX are the same. Kugler and Turk[26]developed a Cellular Automaton model for the simulation of multi-stage deformation and post-dynamic recrystallization for the case when DRX is initiated in the material during deformation. The model enables both quantitative and topological simulations of microstructural evolution before and during PDRX, and it allows the simulation of multi-stage deformation. However, the evolution of the recrystallized grain size was again not considered in the model. The explicit representation of microstructures includes much more information relying on the topological aspects, but when dealing with 3D microstructures with a statistical number of grains, these methods usually become computationally demanding.

Coupled models taking into account recovery, precipitation and recrystallization were also developed[27,28]. Numerical models

[29–31]accounting for recrystallization during and after hot defor-mation for aluminum alloys were developed, such as the ‘‘Through Process Model’’ for the production processes of aluminum[32]. It should be noted that, different from austenitic stainless steels, alu-minum alloys are of high stacking fault energy and recrystalliza-tion is characterized by the gradual formarecrystalliza-tion and appearance of a new structure with no identiﬁable nucleation and growth stages. In general, although some efforts have been reported in model-ing recrystallization durmodel-ing multi-pass conditions for steels, the literature lacks accurate recrystallization models which are able to give quantitative agreements with experimental data (especially grain size) under multi-pass conditions. Most of these models either lack experimental validation or only provide qualitative agreement for selected deformation conditions. The connections between DRX, PDRX, SRX, and grain growth are usually oversimpli-ﬁed. Even though successful prediction of ﬂow stress is usually obtained, the evolution of microstructure in terms of recrystallized fraction and grain size are mostly left unexploited. Furthermore, most of these models are not designed to operate under variable thermal and/or mechanical conditions, therefore making it difﬁcult to use for industrial applications.

In the current work, a physically based numerical model was developed to predict the microstructural evolution during and after hot deformation at the grain scale. The framework of this model is based on a DDRX model[33] published by the current authors where the data structure is represented by a set of repre-sentative grains characterized by two state variables: grain size and dislocation density. Each representative grain is surrounded by two homogeneous equivalent media with high and low dis-location densities representing the average of recrystallized and non-recrystallized grains, respectively. The relative volume weights of the two media are related to their volume fractions,

which represent a new way of introducing topological information into a DDRX model. The key phenomena like strain-hardening, recovery, nucleation of recrystallization occurring during deforma-tion are described with tradideforma-tional equadeforma-tions. The data structure varies with time due to nucleation and disappearance of grains until a steady-state is reached. This results in a two-site mean ﬁeld model with automatic and accurate account of initial grain size effects.

In this paper, signiﬁcant improvements and modiﬁcations have been made to the original DDRX model in order to account for the subsequent PDRX, making the model compatible with recrystal-lization after deformation. This is detailed in Section2. The identi-ﬁcation of model parameters is discussed in Section 3. The predictive capabilities of the model are then validated against 304L stainless steel experimental results in Section4. The model predictions are in excellent quantitative agreement with the experimental observations under different conditions.

2. Model description

The model is presented as follows. Firstly, representation of the microstructure with two-site mean ﬁeld media is described in Section2.1. The general equations describing the key physical phe-nomena occurring during recrystallization are presented from Sections 2.2–2.4, covering the evolution of dislocation density, grain boundary migration and nucleation. Except the static recov-ery equation, these equations were used in our dynamic recrystal-lization model[33], the interested reader is referred to the original publication for more details. A more general expression of the criti-cal dislocation for dynamic recrystallization is proposed in Section2.5, still taking into account of the effect of dynamic recov-ery. The microstructure after deformation is reclassiﬁed according to the dislocation density of the grains, the details of which can be found in Section2.6. A new formulation describing the interaction of the representative grains with the two surrounding Homogeneous Equivalent Medias (HEMs) is shown in Section2.7, where the topological information can be incorporated due to the introduction of the two-site mean ﬁeld media. Finally, the attrac-tive features of this model and its limitation are listed in Section2.8.

2.1. Microstructure representation

The framework is based on a mean ﬁeld approach[33], where each representative grainGi, deﬁned by two state variables (the

grain diameterDiand the grain average dislocation density

q

i), isimmersed in two HEMs (see Fig. 1). A representative grain Gi

accounts for a numberNiof identical spherical grains located at

dif-ferent positions in the microstructure. The neighbors of a given grain in a real recrystallizing microstructure (Fig. 1a) are replaced by two HEMs, respectively referring to the average of recrystallized (RX) and non-recrystallized (NR) grains (Fig. 1b).

The initial set of representative grains typically follows a log-normal distribution for the grain size and a Gaussian distribution for the dislocation densities. However, it has been tested that other distributions can also be used with negligible effect on the ﬁnal result.

2.2. Modeling the evolution of the dislocation density and ﬂow stress

The model makes use of the modiﬁed Kocks and Mecking equa-tion[34–36]to describe the evolution of the dislocation density during deformation

@

q

whereK1(

e

_) andK2(T,e

_) represent, respectively, the strainharden-ing and recovery terms.

The ﬂow stress

r

i is calculated from its average dislocationdensity using the Taylor equation[37]:

r

i¼r

0þMal

b ﬃﬃﬃﬃﬃq

ip

ð2Þ

where

r

0a ‘‘dislocation-free’’ yield stress,Mthe Taylor factor,a

is aconstant set to 0.2,

l

is the shear modulus, and b the Burger’s vector.During post-dynamic recrystallization and subsequent grain growth, the model assumes that the dislocation density of repre-sentative grains can evolve in two different ways, namely due to static recovery and grain growth. Static recovery is only tempera-ture dependent and it is incorporated into the model in a basic way by settingK1in(1)to zero and introducing the static recovery

termKSsuch that, d

q

dt ¼ Ks

q

ð3ÞOnce deformation stops, a slightly deformed grain can still grow at the expense of more severely deformed ones, the area that was just swept by the moving boundary is almost dislocation free. While the total amount of dislocations existing in the growing grain is not affected by this volume change, the average dislocation density in the grain decreases due to the increase of its total volume,

D

ðq

VÞ ¼0D

q

q

¼D

V V ð4Þ2.3. Modeling of grain boundary migration

The driving forceDEfor each grain boundary migration takes into account of the stored energy due to the dislocation content

[2], a capillarity term[38] related to the grain boundary energy and curvature, and the pinning effects:

D

E¼s

D

q

þc

bD

1

r Eth ð5Þ

where

s

l

b2_{/2 is the average energy per unit dislocation length,}

c

b

the energy of the grain boundary per unit area,r=D/2 is the grain radius, andEth is a threshold energy which accounts for pinning

effects. Dq and D(1/r) consider the differences in dislocation density and grain size on either side of the boundary, respectively. The grain boundary velocity evolves according to the kinetic relation[2]

v

¼mD

E ð6Þwheremis the grain boundary mobility. In the present model, the mobility term is included in theK3parameter, given by:

K3¼m

s

ð7Þ2.4. Nucleation model

Within certain grains where the dislocation density is greater than a critical value

q

cr,new grainswill appear due to nucleation.The nucleation rate for theith representative grain is calculated in(8) _ Ni;nucl¼KgScr Nirqið

q

iq

crÞ bg P qk>qcrNkr q kiðq

kq

crÞ bg; Kg¼KgðT; _e

Þ ð8ÞwhereKgis a probability coefﬁcient related to the

thermo-mechani-cal conditions, andScrthe total surface area of grains with

q

>q

cr.Considering that the amount of activated nucleation sites per unit time increases with increasing dislocation density and grain size, the nucleation rate is further normalized by these two items. On the right side of the equation,Niis the number of grains associated

with the ith representative grain. For 304L stainless steel, nucle-ation during DDRX is only assumed to occur at grain boundaries through necklace-type nucleation, hence the valueq= 2 was chosen (for bulk nucleation,q= 3), andbgis a constant with a value close to

3[39]. All nuclei are assumed to start with a low dislocation density

q

0.The model assumes that no nucleation occurs during PRDX. Instead, the RX grains with dislocation densities lower than a criti-cal dislocation density created during the last steps of DDRX are considered as RX. The recrystallization kinetics after deformation is determined by the growth of these RX grains.

2.5. Critical dislocation density and nucleus size

A recrystallization nucleus becomes viable when its radius reaches a critical valueru. This corresponds to the condition when

the stored energy of the material is large enough to overcome the capillary force of the nucleus (Bailey–Hirsch),

q

crs

¼2

c

bru ð

9Þ

Renaming some of the parameters in the critical dislocation density equation proposed by Roberts and Ahlblom[40], an approximate value for

q

DRXcr can be expressed as a function of other parameters

of the model:

Fig. 1.Illustration of a recrystallizing microstructure: (a) representative grain surrounded by recrystallized and non-recrystallized grains; (b) using two HEMs to simplify the grain neighborhood.

q

DRX cr ¼ 20K1c

be

_ 3K3s

1=3 ð10ÞIt is observed from(10)that

q

DRXcr is indirectly inﬂuenced by

tem-perature and strain rate through the parameters K3 and K1.

Temperature variation of

q

DRXcr is mainly dictated by K3 through

the temperature dependence of the mobility parameterm in(7). In general, Eq. (10) states that the critical dislocation density increases with decreasing temperature and increasing strain rate which is physically justiﬁed.

However, the critical dislocation density obtained in (10)

neglects dynamic recovery. Therefore, in some cases it may not be an accurate approximation for

q

DRXcr . Dynamic recovery was

taken into account to calculate the critical dislocation density in

(11)(see[33]), however, it was assumed thatK2

q

DRXcr =K1was muchsmaller than 1. In the conditions used in[32], the approximation was appropriate. ln 1K2 K1

q

DRX cr ¼ K2 rue

_ mq

DRX crs

ð11ÞHowever, when considering a wide range of thermo-mechanical conditions,K2

q

DRXcr =K1may become signiﬁcant. Therefore, using theexpression of the critical nucleus sizerugiven by(9),

q

DRXcr is nowsemi-analytically calculated as

q

DRX cr ¼ 2c

be

_ K2 K3s

ln 1K2 K1q

DRX cr 1=2 ð12ÞAn initial value for

q

DRXcr is obtained directly from(10). An iterative

calculation by(12)leads to the converged value of

q

crDRX_{;}

_{used in}

the model.

To overcome the problem that a nucleus may shrink soon after its creation according to(9), a scaling constant

x

is introduced,rDRX u ¼

x

2c

bq

DRX crs

ð13Þwhere

x

> 1. This will ensure that a created nucleus has the required driving force for growth.2.6. Microstructure reclassiﬁcation

If the strain applied during the deformation stage is beyond

e

DRXcr , dynamic recrystallization will occur. In terms of the resulting

set of representative grains during PDRX, the microstructure can be classiﬁed into four categories (Instead of three categories in[41]) due to the two-site mean ﬁeld approach:

i. DRX nuclei with a dislocation density

q

i=q

0.ii. Growing DRX grains with

q

0<q

i<q

DRXcr .iii. Critically work hardened DRX grains with

q

i>q

DRXcr .iv. Critically work hardened NR grains with

q

i>q

DRXcr .Each of these grain categories will act differently during the sub-sequent annealing process. For example, critically work hardened RX grains will interact with their neighboring grains in a similar way as NR grains; hence, these grains should be considered as NR grains in the following step. In order to be able to describe the different mechanisms and interactions acting in the microstructure after the interruption of deformation, a reclassiﬁcation of the dynamically recrystallized grains is required. In this work, representative grains are reclassiﬁed according to their dislocation densities.

The need to reclassify the microstructure in terms of dislocation
density is illustrated through an EBSD analysis.Fig. 2shows the
inverse pole ﬁgure map and the kernel average misorientation
(KAM) map for a sample deformed at 1000°C up to a strain of
1.5 at a strain rate of 0.1 s1_{. The four types of representative grains}

listed above can be clearly observed inFig. 2b. Small blue grains correspond to type 1 representative grains, while ﬁne green small grains (not the green areas inside the large deformed grains) have the characteristic description of type 2 representative grains. Type 3 grains can be observed in the top left corner in an orange-red color. NR strain-hardened grains (type 4) show a concentration of the deformation at the grain boundaries, where nucleation is observed to occur.

To reclassify the microstructure, we introduce a dislocation density threshold

q

thdeﬁning the limit between RX and NR grains.The value of

q

this chosen to be the maximum dislocation densityobtained when generating the initial dislocation density

Fig. 2.Microstructure obtained after a deformation of 1.5 at a strain rate of 0.1 s1

distribution (Gaussian distribution) for the starting (annealed) microstructure. When there is a change in the recrystallization regime, the representative grains with a dislocation density higher than

q

thare classiﬁed as NR grains.On the other hand, during PDRX the dislocation density of NR grains can be reduced due to both the effect of static recovery and grain growth, as described in Section2.2. If during the holding time a NR representative grain reaches a dislocation density lower than

q

th, this grain will be automatically reclassiﬁed as RX.The advantage of re-deﬁning RX and NR grains as a function of their dislocation density is that the description of the microstruc-ture is simpliﬁed: there is no need to separately identify work hardened old grains and critically work hardened recrystallized grains. Another important beneﬁt of re-deﬁning RX and NR grains lies in the fact that representative grains exhibiting similar behav-ior are grouped accordingly, improving the approximation obtained through the use of 2 HEMs.

2.7. The interaction between representative grain and its surrounding HEMs

In an attempt to describe the neighborhood, two different HEMs surround each representative grain were used: one with a high dis-location density and the other one with a low disdis-location density. Therefore, one part of the boundary for whichDEis high will move faster than the other part, leading to the existence of mobile sur-face fractions[25,32,38]. A schematic representation of this con-cept is shown inFig. 3. The ﬁrst one corresponds to the mobile fraction

c

RXof a RX representative grain. The second one,c

NR isthe mobile fraction of a NR representative grain.

It is convenient to use indicesiandjto designate RX and NR grains, respectively, in the following equations. The driving forces between a representative grain and each HEM are distinguished using the notationDEHEM

k ¼EHEMEkEth;with HEM = NR or RX, k=iorj, andE=

sq

+c

b/r.Due to the different type of interactions and driving forces occurring during the two recrystallization regimes included in the model, two different methods were used to calculate the mobile surface fractions. The ﬁrst formulation is used whenever the dislocation density distribution among grains of the same cate-gory is very narrow. Therefore, it can be assumed that the driving

forces acting between each representative grain with its own HEM are negligible. In this case, the evolution of the microstructure is controlled by the interaction of the representative grains with their opposite HEM. This situation arises during the modeling of DDRX, and is the reason why a simpliﬁed expression for the migration of the different interfaces can be used during this recrystallization regime. The detailed information can be found in Ref.[33].

After DDRX however, the microstructure is composed of four different types of grains as mentioned in the previous section. Grains are reclassiﬁed at the end of the deformation step in terms of their dislocation density. This results in a very diverse and het-erogeneous set (both in size and dislocation density) of NR repre-sentative grains. Due to this reclassiﬁcation, the interaction between NR grains and the NR HEM can no longer be considered as negligible when modeling PDRX. In order to include this effect into the model, the migration of NR–NR and RX–RX interfaces must be considered when deﬁning the mobile surface fractions.

Similarly to the DDRX case, the calculation of the mobile surface fraction terms starts from the boundary velocity expression (7). Considering the movement of all interfaces appearing in the model, the aggregate variations of recrystallized volume (RX–RX, RX–NR) and non-recrystallized volume (NR–NR, NR–RX) are given by,

D

VRX=NR¼ X RXc

RX_{N}i

D

Vi;RX=NR¼ X RXc

RX_{N}i4

p

r2imD

E NR iD

t ð14:1ÞD

VRX=RX¼ X RX 1c

RX NiD

Vi;RX=RX¼ X RX 1c

RX Ni4p

r2imD

E RX iD

t ð14:2Þ and,D

VNR=RX¼ X NRc

NR_{N}j

D

Vj;NR=RX¼ X NRc

NR_{N}j4

p

r2jmD

E RX jD

t ð14:3ÞD

VNR=NR¼ X NR ð1c

NR_{Þ}

_{N}j

D

Vj;NR=NR¼ X NR ð1c

NR_{Þ}

_{N}j4

p

r2jmD

E NR jD

t ð14:4ÞVolume conservation implies that,

D

VRX=NRþD

VRX=RXþD

VNR=RXþD

VNR=NR¼0 ð14:5ÞCombining(14.1-14.5)leads to,

Fig. 3.Illustration of mobile surface fractions (a) as related to a recrystallized representative grain (cRX), and (b) as related to a non-recrystallized representative grain (cNR).

c

NR_{¼}

c

RX P RXNir2iD

E NR i P RXNir2iD

E RX i PNRNjr2jD

E NR j þ P RXNir2iD

E RX i P NRNjr2jD

E RX j P NRNjr2jD

E NR j ð15Þor,

The overall volume change due to boundary migration alone can be expressed by,

D

Vi¼c

RXD

Vi;RX=NRþ ð1c

RXÞD

Vi;RX=RX ð17ÞD

Vj¼c

NRD

Vj;NR=RXþ 1c

NR

D

Vj;NR=NR ð18ÞThe current model assumes that no nucleation occurs during PDRX. Instead, the RX grains with low dislocation densities created during the last steps of DDRX are considered as nuclei and allowed to grow. Although still located along the grain boundaries of strain-hardened grains, these newly created nuclei are in reduced number density such that they do not form a continuous necklace along the grain boundaries. They can be thus considered as randomly distributed in space. Therefore, it can be assumed that the evolution of the

c

RX_{mobile surface fraction can be related to the increase of the}

recrystallized fraction such that

c

RX_{ﬃ}

_{1}

_{}

_{X}

_{ð}

_{19}

_{Þ}

Similarly, considering this time the non-recrystallized volume, one ﬁnds that

c

NR_{ﬃ}

_{X}

_{ð}

_{20}

_{Þ}

Analogous to the previous model for DDRX[33], relations(19) and (20) must however satisfy the volume conservation constraints expressed by(15) and (16). To ensure volume conservation, possi-ble strategies are to either evaluate

c

RX_{from Eq.}

_{(19)}

_{and compute}

c

NR_{using Eq.}

_{(15)}

_{or evaluate}

c

NR_{from Eq.}

_{(20)}

_{and compute}

c

RXwith Eq.(16). The chosen strategy goes as follows. At the beginning of the PDRX process, it is assumed that RX grains are isolated. Thus, at the very beginning

c

RX_{¼}

_{1 and}

c

NR_{is calculated using Eq.}

_{(15)}

_{.}

Once

c

NR_{reaches a value of 1 its value is ﬁxed and the evolution}

of

c

RX_{is calculated using Eq.}

_{(16)}

_{. Volume conservation is thus}

ensured through this switching procedure.

2.8. Attractive features of the model and limitations

From the above description, it can be summarized that the mer-its of the proposed model lie in:

(1) The ability of predicting recrystallized fraction, grain size and ﬂow stress at the same time, with reduced computation cost.

(2) Providing topological information from the interaction of representative grains with two homogeneous equivalent media (two-site approach), which leads to an automatic and accurate account of initial grain size effects.

(3) An easy identiﬁcation of model parameters from experi-ments, the parameters being independent from the initial grain size.

This model also has a number of limitations:

(1) The model is designed for the recrystallization during and after deformation of low stacking fault FCC materials. With only one dislocation density type to describe the internal state of the material during deformation and

recrystallization, the model is not able to adequately describe the cell structure or sub-grains frequently observed for high stacking fault FCC materials like aluminum alloys. The effect of precipitation and second-phase particles is also not considered.

(2) It is based on a grain scale approach. The heterogeneity in terms of the distribution of stored energy and the spread in misorientations within each grain is not yet considered. Nucleation at heterogeneous sites, e.g. through particle stimulated nucleation (PSN), or at shear bands, is neglected. (3) Finally, the model assumes that all grains have the same grain boundary mobility and they follow the same dis-location density evolution law. The model does not take into account the different grains crystallographic orientations and the associated differences in material properties.

3. Parameter identiﬁcation

In order to describe the physical behavior of the material during DDRX, the model makes use of four uncertain parameters: K1

(strain hardening),K2 (dynamic recovery), K3 (mobility), andKg

(nucleation). It is assumed that these parameters are dependent on strain rate and temperature (Except forK1which only depends

on strain rate); therefore, these parameters are identiﬁed in a point-by-point basis in the temperature/strain rate space. Once the parameters are identiﬁed in such a grid of points, intermediate values are determined using a bilinear interpolation.

The value for these parameters can be identiﬁed through purely numerical methods[33]. This approach yields multiple solutions in the form of Pareto optimal sets. However, it was found that some of the solutions failed to describe the PDRX behavior during multi-pass simulations. In PDRX, the evolution of the RX fraction is deter-mined by the growth of RX grains created in the last stages of DDRX. The velocity of the grain interfaces controls this growth, which is a function of dislocation densities and the of boundary mobility. Also, since the volume of the system remains constant, the evolution of the recrystallized grain size during PDRX depends on the number of grains considered as RX. The number of grains contained in each dynamically created representative grain is determined through the parameterKg. Thus, it was concluded that

selecting parameters based only on the values obtained from DDRX data through numerical optimization was not sufﬁcient.

One important aspect of the model is that depending on the parameters used, the mobile surface fraction terms

c

NRand

c

RXmight present instabilities. The model reﬂects the physics of DDRX and PDRX as long as the following conditions are met[33],

d

c

NRdX >0 ð21Þ

d

c

RXdX <0 ð22Þ

If these conditions are not met when using a given set of parame-ters, it is an indication that the model is simulating an unphysical behavior and a different set of parameters must be used.

To solve the problem of multiple solutions leading to unphysi-cal or unstable behaviors, it is required to decrease the degrees

c

RX_{¼}

c

NR P NRNjr2jD

E RX j P NRNjr2jD

E NR j PNRNjr2jD

E NR j þ P RXNir2iD

E RX i P RXNir2iD

E NR i P RXNir2iD

E RX i ð16Þof freedom in the system in order to restrict the solutions to a set of physically consistent values. This was done by obtaining a ﬁrst approximation for the parameters from different recrystallization regimes (where each parameter could be measured experimen-tally). By doing this it was possible to discard unphysical solutions and obtain a set of parameters that actually describes the physical behavior and evolution of the material.

3.1. Strain hardening and recovery: K1and K2

The evolution of the dislocation density during deformation is controlled by the strain hardening termK1and the dynamic

recov-ery term K2. The ﬁrst approximation for these values can be

obtained through the stress strain curves.

Starting from the integration of(1)the description of the ﬂow curve is given by[42],

r

¼r

2sat ð

r

2satr

02ÞexpðK2e

Þ1=2

ð23Þ

where

r

0 andr

sat represent the yield stress and the saturationstress respectively.

r

satdepends onK1andK2according to,r

sat¼Mal

b ﬃﬃﬃﬃﬃﬃ K1 K2 s ð24ÞSince the ﬂow stress is given by(2), it is possible to rewrite(1)in terms of the ﬂow stress such that,

@

q

@e

¼ ðMal

bÞ 2dr

2 de

¼2ðMal

bÞ 2r

dr

de

ð25ÞBy combining(2) and (25), the evolution Eq.(1)can be rewritten as,

2

r

h¼K2r

sat2 K2r

2 ð26Þwhereh=d

r

/de

is the current work hardening rate. The parameterK2 is obtained from the slope (K2) of the 2h

r

vs.r

2 from theexperimental ﬂow stress curves.K1is obtained fromK2using,

K1¼ K2

r

2satðM

al

bÞ2 ð27Þ3.2. Grain boundary mobility: K3

Due to the different mechanisms occurring during DDRX, obtaining the accurate value forK3 proves to be a difﬁcult task.

Instead, a lower bound ﬁrst approximation for this parameter is obtained through grain growth experiments. It is assumed that mobility is the lowest during grain growth and increases as a func-tion of strain rate for a given temperature.

Grain growth is directly linked to the grain boundary mobility through(7). To estimate the lower bound forK3, the model was

ﬁt-ted against pure grain growth experiments. This was done by generating a dislocation free grain size distribution and monitoring the curvature driven evolution of the different representative grains. The parameter K3 was then manually calibrated so that

the model could ﬁt the experimental data. This was done once for each temperature.

3.3. Nucleation: Kg

The nucleation rate parameterKgis perhaps the most difﬁcult

parameter to measure experimentally. For this reason, this parameter is the last one to be calibrated and must be done by run-ning a DDRX-PDRX simulation. After ﬁnding a set of parameters (K1,K2, andK3) that correctly describes the DDRX behavior,Kgis

obtained by ﬁtting the kinetics and the grain size in the PDRX regime.

This cross-regime validation for parameter values is a method that insures and allows the model to simulate multi-pass processes using a natural set of parameters, increasing its predictive capabilities.

4. Model validation

The progress of the DDRX and PDRX can be directly measured
from metallographic examination. However, very limited
recrystal-lized fraction and grain size data are available in the literature. The
vast majority of existing data focuses only on the softening
frac-tion, which is the combined effect of both recrystallization and
recovery if precipitation is absent. For the validation of the model,
304L austenitic stainless steel was chosen. To improve the
accu-racy, microstructures at different conditions were characterized
by EBSD to determine the recrystallized volume fraction and grain
size. Two test cases of hot deformation followed by a holding time
at the same temperature were performed. This was done to
ana-lyze DRX, PDRX, and grain growth at the same time. The relative
values of the ﬁtting parameters used for 304L stainless steel are
listed inAppendix B. Parameters are expressed in a dimensionless
form, relative to reference values obtained at 0.01 s1_{and 1000}_{°}_{C.}

For the PDRX/GG regime,K1andKgare both set to zero, since no

deformation and nucleation of recrystallization are involved. And the dynamic recovery term K2 is replaced by static recovery Ks.

As can be seen fromFig. B-1,K1,K3andKgincrease with strain rate

whileK2decreases with strain rate, which are physically justiﬁed.

The model was tested at different temperatures and strain rates for the different recrystallization regimes, however, only the results obtained at 1000°C are presented in this paper. For these simulations, the initial number of representative grains was set to 50.

4.1. Experimental methods and thermo-mechanical treatment

The 304L stainless steel torsion samples used had a gauge length of 15 mm, a diameter of 6 mm, and were machined from rolled bars. Hot torsion tests were performed according to the schematic diagram illustrated in Fig. 4. In order to achieve a homogeneous distribution of the temperature and avoid thermal ﬂuctuations, the samples were held for 3 min after reaching the target temperature T0: The initial grain size was 135

l

m. Thesamples were then deformed at the temperatureT0(1000°C) to

different strains, at strain rates of 0.01 and 0.1 s1

. After the desired strain or holding time had been reached, samples were water-quenched to room temperature.

Fig. 4.Schematic diagram of torsion test for investigation of different recrystallization.

Samples were then polished for microscopy analysis following a standard metallographic preparation: successive wet grinding starting from a 600 grit paper until 4000 grit, and a ﬁnal polishing stage using colloidal silica to obtain a well ﬁnished surface. For EBSD analysis, the samples were subjected to an additional vibra-tory polishing for 6 h. For optical microscopy (OM) analysis, the polished samples were etched by a chemical solution composed of 50 ml hydrochloric acid (HCl) and 15 drops of H2O2 (5 ml).

Metallographic observations were performed on tangential sec-tions at a depth of100

l

m below the sample surface.4.1.1. Dynamic recrystallization

The comparison between the experimental results and those predicted by the model for DDRX are presented inFig. 5. The model accurately describes the evolution of the recrystallized fraction in both cases. The ﬂow stress as a function of the strain is shown in

Fig. 5a. The increase in the ﬂow stress due to an increase in strain
rate is well captured by the model. It can be observed fromFig. 5b,
both numerically and experimentally, that recrystallization
kinet-ics is faster for the test case using a strain rate of 0. 01 s1_{. The }

evo-lution of grain size combined with strain rate affects the shape of the ﬂow stress curves (seeFig. 5c), and leads to a decrease in the peak stress and steady state stress.

In terms of ﬂow stress, recrystallized fraction and grain size, there is a very good agreement between the experimental results and those predicted by the model. This good agreement shows that the identiﬁedKparameters are physically consistent and describe correctly the mechanisms observed during DDRX. As mentioned in the parameter identiﬁcation section, the parameters values have to be validated against PDRX. This is done by making a coupled sim-ulation, modeling PDRX and grain growth after DDRX.

4.1.2. Post-dynamic recrystallization

The model was validated against two test cases during PDRX.
Samples were deformed at 1000°C up to a strain of 1.5, at a strain
rate of 0.01 s1 _{and 0.1 s}1 _{respectively. After deformation,}

samples were held at the same temperature of 1000°C for different holding times before they were water quenched to room temperature.

To determine the RX fraction during DDRX, experimental
results obtained by OM or EBSD can be directly compared to those
of the model. For PDRX however, additional considerations must be
taken. At the beginning and during PDRX, the model reclassiﬁes
representative grains as RX or NR in terms of their dislocation
density. In order to compare the recrystallized volume fractions
predicted by the model to those observed experimentally, the
ker-nel average misorientation (KAM) maps obtained through EBSD
were employed.Fig. 6shows the microstructure after hot
deforma-tion to 1.5 at 1000°C with a strain rate of 0.01 s1_{and with 60s’}

holding time before quick water quench. With the exception of a few elongated grains, Fig. 6a shows a fully recrystallized microstructure. However, after analyzing the microstructure using KAM maps (not the same observed area as OM images) obtained by EBSD, it is observed that some small grains have non-negligible stored energy. These grains were most likely created during DDRX (type 2 and 3) and have a similar size and shape as those which are fully recrystallized, shown in blue in Fig. 6b. The RX kinetics in PDRX is determined by the growth of grains with a dis-location density close to

q0

toward the deformed matrix, and the latter includes small grains created during DDRX.The comparison between the recrystallization kinetics
mea-sured experimentally by EBSD and those obtained with the model
during PDRX at 1000°C after a deformation of 1.5 with two strain
rates of 0.01 s1 _{and 0.1 s}1 _{is presented in}_{Fig. 7}_{. It should be}

noted that at the beginning of the PDRX process, the recrystallized fraction is close to zero, this is because only a small part of the RX

grains (nucleated recently) after DRX has a dislocation density less than

q

th, other RX grains get strained quickly. The model shows anoverall good agreement for the two cases, the fact that recrystal-lization kinetics is faster when the strain rate is higher is also cap-tured, but there is a slight underestimate of the recrystallized volume fraction. Since the model assumes PDRX occurs only due to the growth of dynamically created nuclei with a dislocation den-sity lower than

q

_{th}, at least part of the differences can be attributed to some type of secondary nucleation occurring in the microstruc-ture due to SRX.

The evolution of the recrystallized grain size during PDRX for the same test cases is presented inFig. 8. The model captures the

Fig. 5.Comparison between experimental and numerical results obtained with the
model (DRX) (a) ﬂow stress curves, (b) recrystallized fraction, (c) recrystallized
grain size. Conditions are at 1000°C,e= 0.01 s1_{and 0.1 s}1_{respectively.}

evolution accurately. Also, two distinct regimes can be observed, in accordance with existing literature[43,44]. At the beginning, there is a fast evolution of the grain size. This is due to the fast growth of nuclei created during the last stages of DDRX. The driving force for this growth is primarily due to the difference in dislocation density between the deformed grains and those with a dislocation density close to

q0

. As the microstructure approaches a fully recrystallized state, the driving force and hence the grain growth rate decrease, leading to the plateau observed between 100 and 800s. Once themicrostructure is fully recrystallized, normal grain growth occurs, and the driving force controlling the evolution is due to the curva-ture of the grains. The model is able to capcurva-ture completely this two-step behavior observed experimentally.

In general, the model is able to give both qualitative and quan-titative agreements between experimental results and predicted ones in terms of ﬂow stress, recrystallized fraction and recrystal-lized grain size during and after hot deformation at different pro-cessing conditions. Considering its inherent simplicity, this model

Fig. 6.Micrographs of a torsion sample deformed at 1000°C with a strain rate of 0.01 s1

to a strain of 1.5 and held for 60s before water quench. (a) Micrograph obtained with Optical microscopy, (b) micrograph obtained with EBSD, color coded related to Kernel Average Misorientation. (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

Fig. 7.PDRX kinetics after a deformation of 1.5 at 1000°C with: (a) strain rate of 0.01 s1

, and (b) strain rate of 0.1 s1 .

Fig. 8.Evolution of the PDRX recrystallized grain size after deformation of 1.5 at 1000°C with: (a) strain rate of 0.01 s1

, and (b) strain rate of 0.1 s1 .

can be easily implemented into a ﬁnite element software for indus-trial application, since it provides a satisfactory description of dif-ferent phenomena occurring during and after hot deformation. It is believed that the model has sufﬁcient generality to be directly used for other materials with low stacking fault energy. It could also be extended to other types of materials by changing the nucleation model and/or the evolution equations of mobile surface fractions reﬂecting the topological description. Further efforts are being invested to improve the current model, including the analysis of the grain size distribution, the relationship between ﬂow stress and recrystallized grain size during DDRX [45], and the strain independent characteristics of the softening associated with PDRX once a certain prestrain is attained[46]. Meanwhile, a wider range of experiments are planned to provide sufﬁcient data for model calibration.

5. Conclusions

A model describing recrystallization in metallic materials cap-able of handling DRX, PDRX, and grain growth was developed and validated against experimental test cases for multi-pass hot deformation of 304L austenitic stainless steel. The focus of this work was to develop a numerical model able to predict microstruc-tural evolution due to different recrystallization regimes. The key physical ingredients of this model are: a modiﬁed Kocks– Mecking equation to follow the evolution of dislocation density, a time dependent nucleation law taking into account dynamic recovery, non-constant growth rates, and topological information coming from the introduction of two HEMs. The proposed model has been able to provide quantitative predictions of the recrystal-lized fraction, the recrystalrecrystal-lized grain size, and the ﬂow stress curves for different conditions: a good indication that the basic mechanisms of recrystallization during and after deformation are well captured by the model. This simple model can therefore be considered as a tool for the optimization of thermomechanical pro-cessing at the industrial scale.

The method to determine the values of the parameters used by the model is also described. By obtaining and validating the parameters from different experimental data in different recrystal-lization regimes, parameter tuning becomes efﬁcient. This also solves the problem of obtaining multiple solutions lacking a physi-cal meaning. By using parameters obtained with such a methodol-ogy, the model is stable and its predictive capabilities are increased.

Appendix A. List of symbols used

The following notation is used in the article, some of the sym-bols were already used in[33].

b Burger’s vector (m)

bg constant related to nucleation

s

energy per unit dislocation length (N)m grain boundary mobility (m3_{s}1_{N}1_{)}

d0;D0 initial average grain diameter (m) dss steady state grain size

ddrx dynamically recrystallized grain size

dpdrx post-dynamically recrystallized grain size

Dmax initial maximum grain diameter (m)

DRX average grain diameter of recrystallized grains (m)

K1 parameter related to strain hardening (m2) K2 parameter related to dynamic recovery Ks parameter related to static recovery

K3 parameter related to grain boundary mobility

(m3_{s}1_{),}_{K}
3=m

s

Kg probability parameter related to nucleation (m2s1)

Ks static recovery parameter

M Taylor factor

Np number of potential nucleation sites

_

Nnucl total number of activated nuclei per unit time (s

1

)

q parameter related the type of nucleation (surface or volume)

r grain radius (m)

g

constant for grain growthn grain growth exponent

rRX recrystallized grain radius (m)

rDRX

u radius of a DRX nucleus (m)

rSRX

u radius of a SRX nucleus (m)

rHEM radius of homogeneous equivalent media (m)

x

scaling constant for SRX/DRX nucleusDE driving force for grain boundary migration

Ez grain boundary migration pinning

Scr surface area of all grain boundaries satisfying

q

>q

cr(m2)X recrystallized volume fraction

q

i dislocation density of representative graini(m2)q

0 Initial average dislocation density (m2)q

max initial maximum dislocation density (m2)q

DRXcr ;

q

cr critical dislocation density for DRX (m2_{)}

q

HEM dislocation density for the homogenous equivalentmedia

q

SRXcr critical dislocation density for SRX (m

2

)

q

SRVss minimal dislocation density for static recovery

(m2_{)}

q

th critical dislocation density for re-deﬁning RX andNR grains (m2_{)}

b constant to relate

q

Discr and

q

SRXcre

strain or deformatione

DRXcr ;

e

cr critical strain for DRXr

i ﬂow stress of representative graini(MPa)r0

dislocation free yield stress (MPa)

r

macroscopic ﬂow stress (MPa)l

shear modulus (MPa)E elastic modulus (MPa)

m

Poisson’s ratioa

constant related to ﬂow stressc

b grain boundary energy per unit area (J m2)v

grain boundary velocity (m s1_{)}

_

e

strain rate (s1_{)}

c

RX_{mobile surface fraction of a recrystallized}

representative grain

c

NR_{mobile surface fraction of non-recrystallized}

representative grain

Z _{Zener–Hollomon parameter}_{Z}_{¼}

e

_expðQ=RTÞc

SFE stacking fault energyAppendix B. Relative value for the ﬁtting parameters Fig. B-1.

References

[1]J.W. Christian, The Theory of Transformations in Metals and Alloys, third ed., Pergamon Press, Oxford; New York, 2002. pp. 851.

[2]F.J. Humphreys, M. Hatherly, Recrystallization and Related Annealing Phenomena, Second ed., Elsevier, Oxford, 2004.

[3]G.A. Wilber, J.R. Bell, J.H. Bucher, W.J. Childs, TMS-AIME 244 (1968) 2305– 2308.

[4] A. Dehghan-Manshadi, The evolution of recrystallization during and following hot deformation. Ph.D thesis, Deaking University, Australia, 2007.

[5]R.A.P. Djaic, J.J. Jonas, J. Iron Steel Inst. 210 (1972) 256–261. [6]R.A. Petkovic, M.J. Luton, J.J. Jonas, Acta Metall. 27 (1979) 1633–1648. [7]M.J. Luton, R.A. Petkovic, J.J. Jonas, Acta Metall. 28 (1980) 729–743. [8]Z. Xu, T. Sakai, Mater. Trans. JIM 32 (1991) 174–180.

[9]T. Sakai, M. Ohashi, K. Chiba, J.J. Jonas, Acta Mater. 36 (1988) 1781–1790. [10]P.D. Hodgson, R.K. Gibbs, ISIJ Int. 32 (1992) 1329–1338.

[11]C. Roucoules, P.D. Hodgson, Mater. Sci. Technol. 11 (1995) 548–556. [12]H. Beladi, P. Cizek, P.D. Hodgson, Acta Materialia 59 (2011) 1482–1492. [13]N. Yazdipour, P.D. Hodgson, Computat. Mater. Sci. 54 (2012) 56–65.

[14]A. Dehghan-Manshadi, M.R. Barnett, P.D. Hodgson, Metall. Mater. Trans. A 39A (2008) 1359–1370.

[15]A. Dehghan-Manshadi, M.R. Barnett, P.D. Hodgson, Mater. Sci. Eng. A 485 (2008) 664–672.

[16]S. Cho, K. Kang, J.J. Jonas, ISIJ Int. 41 (2001) 63–69. [17]S. Cho, K. Kang, J.J. Jonas, ISIJ Int. 41 (2001) 766–773.

[18]A. Kirihata, F. Siciliano, T.M. Maccagno, J.J. Jonas, ISIJ Int. 38 (1998) 187–195. [19]S.H. Cho, Y.C. Yoo, J. Mater. Sci. 36 (2001) 4279–4284.

[20] S.H. Cho, Y.C. Yoo, J. Mater. Sci. 36 (2001) 4267–4272. [21]D.S. Svyetlichnyy, ISIJ Int. 45 (2005) 1187–1193.

[22]B. Radhakrishnan, G.B. Sarma, T. Zacharia, Acta Materialia 46 (1998) 4415– 4433.

[23]C. Roucoules et al., Mater. Sci. Eng. A 339 (2003) 1–9. [24]R. Sandstrom, R. Lagneborg, Acta Metall. 23 (1975) 387–398. [25]R. Sandstrom, R. Lagneborg, Acta Metall. 23 (1975) 481–488. [26]G. Kugler, R. Turk, Acta Materialia 52 (2004) 4659–4668.

[27]H.S. Zurob, Y. Brechet, G. Purdy, Acta Materialia 49 (2001) 4183–4190. [28]H.S. Zurob, C.R. Hutchinson, Y. Brechet, G. Purdy, Acta Materialia 50 (2002)

3077–3094.

[29]H.E. Vatne, E. Nes, Computat. Mater. Sci. 7 (1996) 5–10.

[30] H.E. Vatne, K. Marthinsen, R. Ørsund, E. Nes, Metall. Mater. Trans. A 27A (1996) 4133–4144.

[31]H.E. Vatne, F. Perocheau, H.E. Ekstrom, L. Poizat, E. Nes, J. Hagstrom, M. Lyttle, T. Furu, J. de Physique IV 11 (2001) 123–130.

[32]J. Hirsch, Virtual Fabrication of Aluminum Products: Microstructural Modeling in Industrial Aluminum Production, Wiley-VCH, 2007.

[33]P. Bernard, S. Bag, K. Huang, R.E. Logé, Mater. Sci. Eng. A 528 (2011) 7357– 7367.

[34]U.F. Kocks, J. Eng. Mater. Technol. 98 (1976) 76–85. [35]H. Mecking, U.F. Kocks, Acta Metall. 29 (1981) 1865–1875. [36]Y. Estrin, H. Mecking, Acta Metall. 32 (1984) 57–70. [37]G.I. Taylor, Proc. R. Soc. London Ser. A 145 (1934) 362–387. [38]M. Hillert, Acta Metall. 13 (1965) 227–238.

[39]F. Montheillet, O. Lurdos, G. Damamme, Acta Mater. 57 (2009) 1602–1612. [40] W. Roberts, B. Ahlblom, Acta Metall. 26 (1978). 801-813-209.

[41]T. Sakai, M. Ohashi, Mater. Sci. Technol. 6 (1990) 1251–1257.

[42]X. Quelennec, E. Martin, L. Jiang, J.J. Jonas, J. Phys.: Confer. Series 240 (2010) 012082.

[43]T. Sakai, M. Ohashi, Mater. Sci. Forum 113–115 (1993) 521–526.

[44] T. Sakai, Static recovery, recrystallization and grain growth in dynamically recrystallized materials, Proceedings of ReX’96, the 3rd International Conference on Recrystallization and Related Phenomena, Edited by Terry R. McNelley, 1997, pp. 137–148.

[45]B. Derby, Acta Metall. Mater. 39 (1991) 955–962.

[46]A. Dehghan-Manshadi, J.J. Jones, P.D. Hodgson, M.R. Barnett, ISIJ Int. 48 (2008) 208–211.

Fig. B-1.Relative evolution of K parameters at 1000°C, with respect to the reference values obtained at 0.01 s1